Pressure inverse solubility and polymorphism of an edible γ-cyclodextrin-based metal-organic framework.
Patyk-Kaźmierczak, Ewa; Warren, Mark R.; Allan, David R.; Katrusiak, Andrzej; Physical chemistry chemical physics : PCCP 19 (2017) 9086–9091; doi:10.1039/c7cp00593h

data_7227783
_publ_section_title
;
 Pressure inverse solubility and polymorphism of an edible
 \g-cyclodextrin-based metal-organic framework.
;
_journal_issue                   13
_journal_name_full               'Physical chemistry chemical physics : PCCP'
_journal_page_first              9086
_journal_page_last               9091
_journal_paper_doi               10.1039/c7cp00593h
_journal_volume                  19
_journal_year                    2017
_chemical_absolute_configuration rm
_chemical_formula_moiety         'C48 H80 O40, 2(KOH)'
_chemical_formula_sum            'C48 H82 K2 O42'
_chemical_formula_weight         1409.34
_chemical_name_common            '\g-cyclodextrin-metal-organic framework'
_chemical_name_systematic
'catena-((\m8-\g-Cyclodextrin)-di-potassium dihydroxide)'
_space_group_crystal_system      cubic
_space_group_IT_number           211
_space_group_name_Hall           'I 4 2 3'
_space_group_name_H-M_alt        'I 4 3 2'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_audit_creation_date             2017-01-18
_audit_creation_method
;
Olex2 1.2
(compiled 2017.01.04 svn.r3372 for OlexSys, GUI svn.r5289)
;
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            12
_cell_length_a                   30.968(6)
_cell_length_b                   30.968(6)
_cell_length_c                   30.968(6)
_cell_measurement_reflns_used    361
_cell_measurement_temperature    295
_cell_measurement_theta_max      8.8520
_cell_measurement_theta_min      4.6780
_cell_volume                     29699(10)
_computing_cell_refinement       'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_diffrn_ambient_environment      'diamond-anvil cell'
_diffrn_ambient_pressure         990000
_diffrn_ambient_temperature      295
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.2413
_diffrn_detector_type            Eos
_diffrn_measured_fraction_theta_full 0.732
_diffrn_measured_fraction_theta_max 0.729
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  t~exp~   \w     \q     \k     \f   Frames
--------------------------------------------------------------------------
  1  \f    -35.00  19.75   0.75   20.00   0.00 -30.00   0.00    --    73
  2  \f    140.00 200.00   0.75   20.00   0.00 -30.00   0.00    --    80
  3  \f    160.00 217.00   0.75   20.00   0.00  30.00   0.00    --    76
  4  \f    -20.00  34.75   0.75   20.00   0.00  30.00   0.00    --    73
  5  \w    -24.00  24.00   0.75   20.00    --   30.00  39.46 -12.90   64
  6  \w    -24.00  24.00   0.75   20.00    --   30.00  39.46 167.10   64
  7  \w    -50.00  10.00   0.75   20.00    --  -30.00  39.46 167.10   80
  8  \w    -50.00  10.00   0.75   20.00    --  -30.00  39.46 -12.90   80
  9  \w    -64.00  -8.50   0.75   20.00    --  -30.00  81.40 -28.90   74
 10  \w    -64.00  -8.50   0.75   20.00    --  -30.00  81.40 151.10   74
 11  \w    -19.00   8.00   0.75   20.00    --   30.00  81.40 151.10   36
 12  \w    -19.00   8.00   0.75   20.00    --   30.00  81.40 -28.90   36
 13  \w    -43.00 -21.25   0.75   20.00    --   30.00 134.60 -56.90   29
 14  \w    -43.00 -21.25   0.75   20.00    --   30.00 134.60 123.10   29
 15  \w    -90.00 -36.00   0.75   20.00    --  -30.00 134.60 123.10   72
 16  \w    -90.00 -36.00   0.75   20.00    --  -30.00 134.60 -56.90   72
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0027204000
_diffrn_orient_matrix_UB_12      0.0015446000
_diffrn_orient_matrix_UB_13      0.0226885000
_diffrn_orient_matrix_UB_21      0.0189117000
_diffrn_orient_matrix_UB_22      0.0125009000
_diffrn_orient_matrix_UB_23      -0.0033111000
_diffrn_orient_matrix_UB_31      -0.0126269000
_diffrn_orient_matrix_UB_32      0.0191002000
_diffrn_orient_matrix_UB_33      0.0002382000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.2967
_diffrn_reflns_av_unetI/netI     0.0867
_diffrn_reflns_Laue_measured_fraction_full 0.732
_diffrn_reflns_Laue_measured_fraction_max 0.729
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            7547
_diffrn_reflns_point_group_measured_fraction_full 0.783
_diffrn_reflns_point_group_measured_fraction_max 0.781
_diffrn_reflns_theta_full        10.197
_diffrn_reflns_theta_max         10.197
_diffrn_reflns_theta_min         4.837
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    0.164
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.67886
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.38.41 (Rigaku Oxford Diffraction, 2015)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    0.945
_exptl_crystal_description       plate
_exptl_crystal_F_000             8928
_exptl_crystal_recrystallization_method
'Compressed crystal that was grown in situ from methano:water solution in the diamond-anvil cell at 0.1 GPa.'
_exptl_crystal_size_max          0.17
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.1
_refine_diff_density_max         0.107
_refine_diff_density_min         -0.092
_refine_diff_density_rms         0.024
_refine_ls_abs_structure_details
;
 Flack x determined using 89 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.8(4)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.174
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     75
_refine_ls_number_reflns         264
_refine_ls_number_restraints     75
_refine_ls_restrained_S_all      1.786
_refine_ls_R_factor_all          0.0869
_refine_ls_R_factor_gt           0.0865
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.2000P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2315
_refine_ls_wR_factor_ref         0.2326
_reflns_Friedel_coverage         0.610
_reflns_Friedel_fraction_full    0.884
_reflns_Friedel_fraction_max     0.885
_reflns_number_gt                260
_reflns_number_total             264
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7cp00593h3.cif
_cod_data_source_block           CDMOF_a_0_99GPa
_cod_depositor_comments
'Adding full bibliography for 7227776--7227790.cif.'
_cod_original_cell_volume        29699(11)
_cod_database_code               7227783
_shelx_shelxl_version_number     2014/7
_chemical_oxdiff_formula         'C48 H82 K2 O40'
_reflns_odcompleteness_completeness 82.74
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     10.18
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups
 At 1.5 times of:
  All O(H) groups
2. Restrained distances
 C14-O14
 1.45 with sigma of 0.002
 C14-C13
 1.5 with sigma of 0.02
 O2-C3
 2.2 with sigma of 0.02
 C11-O4
 1.45 with sigma of 0.002
 C11-C14
 3 with sigma of 0.02
 C4-O4
 1.45 with sigma of 0.002
 C4-C3
 1.5 with sigma of 0.002
 C12-O4
 2 with sigma of 0.02
 C12-C13
 1.5 with sigma of 0.02
 C12-C11
 1.5 with sigma of 0.002
 C2-C3
 1.5 with sigma of 0.002
 C2-O2
 1.45 with sigma of 0.002
 C1-C4
 2.8 with sigma of 0.02
 C2-C1
 1.5 with sigma of 0.002
 O3-C3
 1.45 with sigma of 0.002
 C2-O3
 2.3 with sigma of 0.02
 C16-C15
 1.5 with sigma of 0.002
 C14-C15
 1.5 with sigma of 0.002
 O14-C15
 2.4 with sigma of 0.02
 C12-C15
 3 with sigma of 0.02
 C15-C12
 3 with sigma of 0.02
 C6-C5
 1.5 with sigma of 0.002
 C4-C5
 1.5 with sigma of 0.002
 C2-C5
 3 with sigma of 0.02
 C5-C2
 3 with sigma of 0.02
 C5-C1
 2.3 with sigma of 0.002
 C5-C4
 1.5 with sigma of 0.02
 C3-C4
 1.5 with sigma of 0.02
 O4-C4
 1.45 with sigma of 0.02
 C16-O16
 1.45 with sigma of 0.002
 C6-O6
 1.45 with sigma of 0.002
 O13-C13
 1.45 with sigma of 0.002
 C12-O12
 1.45 with sigma of 0.02
 O5-C6
 2.5 with sigma of 0.02
 O15-C16
 2.2 with sigma of 0.02
 O5-C3
 3 with sigma of 0.02
 O15-C13
 3 with sigma of 0.02
 O15-C11
 1.45 with sigma of 0.002
 O5-C1
 1.45 with sigma of 0.002
 O15-C15
 1.45 with sigma of 0.002
 O5-C5
 1.45 with sigma of 0.002
 C13-O14
 2.5 with sigma of 0.04
 C11-C13
 2.4 with sigma of 0.02
 C11-C4
 2.5 with sigma of 0.04
 C12-C14
 2.4 with sigma of 0.02
 O2-C3
 2.5 with sigma of 0.04
 C4-C2
 2.5 with sigma of 0.02
 O4-C3
 2.5 with sigma of 0.04
 O4-C12
 2.5 with sigma of 0.04
 C3-C1
 2.5 with sigma of 0.02
 O2-C1
 2.5 with sigma of 0.04
 C13-C15
 2.4 with sigma of 0.02
 O14-C15
 2.5 with sigma of 0.04
 C15-C11
 2.4 with sigma of 0.02
 C5-C3
 2.5 with sigma of 0.02
 O4-C5
 2.5 with sigma of 0.04
 C1-C5
 2.5 with sigma of 0.02
 C4-C11
 2.5 with sigma of 0.04
 C2-C4
 2.5 with sigma of 0.04
 C5-O6
 2.5 with sigma of 0.04
 O13-C14
 2.5 with sigma of 0.04
 O13-C12
 2.5 with sigma of 0.04
 O12-C11
 2.5 with sigma of 0.04
 C14-O15
 2.4 with sigma of 0.02
 O5-C4
 2.5 with sigma of 0.02
 O15-C12
 2.4 with sigma of 0.02
 C2-O5
 2.5 with sigma of 0.02
 O4-O15
 2.5 with sigma of 0.04
 C4-O5
 2.5 with sigma of 0.04
3. Uiso/Uaniso restraints and constraints
Uanis(K1) \\sim Ueq: with sigma of 0.1 and sigma for terminal atoms of 0.2
4. Others
 Uiso(C1)=Uiso(C2)=Uiso(C3)=Uiso(C4)=Uiso(C5)=Uiso(C6)=Uiso(C11)=Uiso(C12)=
 Uiso(C13)=Uiso(C14)=Uiso(C15)=Uiso(C16)=FVAR(1)
 Uiso(O2)=Uiso(O3)=Uiso(O4)=Uiso(O5)=Uiso(O6)=Uiso(O12)=Uiso(O13)=Uiso(O14)=
 Uiso(O15)=Uiso(O16)=Uiso(OA)=FVAR(2)
5.a Ternary CH refined with riding coordinates:
 C1(H1), C2(H2A), C3(H3A), C4(H4), C5(H5), C11(H11), C12(H12A), C13(H13A),
 C14(H14), C15(H15)
5.b Secondary CH2 refined with riding coordinates:
 C6(H6A,H6B), C16(H16A,H16B)
5.c Tetrahedral OH refined with riding coordinates:
 O2(H2), O3(H3), O6(H6), O12(H12), O13(H13), O16(H16)
;
_olex2_exptl_crystal_mounting_method 'Diamond-anvil cell'
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.000
_oxdiff_exptl_absorpt_empirical_full_min 1.000